π-extended tetrathiafulvalene and its charge-transfer ... · π-extended tetrathiafulvalene and...
Embed Size (px)
Transcript of π-extended tetrathiafulvalene and its charge-transfer ... · π-extended tetrathiafulvalene and...
Single-molecule conductance of a chemically modified,-extended tetrathiafulvalene and its charge-transfer complexwith F4TCNQRal Garca1, M. ngeles Herranz1, Edmund Leary*2, M. Teresa Gonzlez2,Gabino Rubio Bollinger3, Marius Brkle4, Linda A. Zotti5, Yoshihiro Asai4, Fabian Pauly6,Juan Carlos Cuevas5, Nicols Agrat2,3 and Nazario Martn*1,2
Full Research Paper Open AccessAddress:1Departamento de Qumica Orgnica, Facultad de Qumica,Universidad Complutense, E-28040 Madrid, Spain, 2FundacinIMDEA Nanoscience, Campus de Cantoblanco, UniversidadAutnoma, E-28048 Madrid, Spain, 3Departamento de Fsica de laMateria Condensada, and Instituto Nicols Cabrera, UniversidadAutonoma de Madrid, E-28049 Madrid, Spain, 4NanosystemResearch Institute, National Institute of Advanced Industrial Scienceand Technology (AIST), Tsukuba, Ibaraki 305-8568, Japan,5Departamento de Fsica Terica de la Materia Condensada,Universidad Autnoma de Madrid, Spain and 6Department of Physics,University of Konstanz, D-78457 Konstanz, Germany
Email:Edmund Leary* - [email protected]; Nazario Martn* [email protected]
* Corresponding author
Keywords:break junction measurements; charge-transfer complex; DFT-basedtransport; molecular electronics; tetrathiafulvalene
Beilstein J. Org. Chem. 2015, 11, 10681078.doi:10.3762/bjoc.11.120
Received: 11 March 2015Accepted: 22 May 2015Published: 24 June 2015
This article is part of the Thematic Series "Tetrathiafulvalene chemistry".
Guest Editor: P. J. Skabara
2015 Garca et al; licensee Beilstein-Institut.License and terms: see end of document.
AbstractWe describe the synthesis and single-molecule electrical transport properties of a molecular wire containing a -extended tetrathia-fulvalene (exTTF) group and its charge-transfer complex with F4TCNQ. We form single-molecule junctions using the in situ breakjunction technique using a homebuilt scanning tunneling microscope with a range of conductance between 10 G0 down to 107 G0.Within this range we do not observe a clear conductance signature of the neutral parent molecule, suggesting either that its conduc-tance is too low or that it does not form a stable junction. Conversely, we do find a clear conductance signature in the experimentscarried out on the charge-transfer complex. Due to the fact we expected this species to have a higher conductance than the neutralmolecule, we believe this supports the idea that the conductance of the neutral molecule is very low, below our measurement sensi-tivity. This idea is further supported by theoretical calculations. To the best of our knowledge, these are the first reported single-molecule conductance measurements on a molecular charge-transfer species.
http://www.beilstein-journals.org/bjoc/about/openAccess.htmmailto:[email protected]:[email protected]://dx.doi.org/10.3762%2Fbjoc.11.120
Beilstein J. Org. Chem. 2015, 11, 10681078.
IntroductionThe development of molecular electronics is a current chal-lenge in nanoscience. The ultimate goal is to fabricate differentelectronic devices based on a variety of active elements such aswires, transistors, diodes or switches (to name just a few),where each is built from individual, suitably functionalizedmolecules. Although the controlled handling of molecules toform reliable molecule-based circuits remains a demandingtask, modern organic synthesis allows the design and prepar-ation of nearly any challenging molecule .
Among the aforementioned electroactive elements, the study ofmolecular wires has received great attention and, in this regard,a great variety of molecules of different nature involving single,double and triple CC bonds (conjugated or not) have beenextensively studied [2-4]. Furthermore, most of these systemshave been covalently connected to a great variety of differentanchor groups in order to improve the connection to variousmetal electrodes. However, despite the huge number of molec-ular systems that find application as wires, the use of electroac-tive molecules exhibiting different oxidation states that canmodify/control the conductance through the wire have beenconsiderably less studied.
In the realm of organic chemistry there are a great variety oforganic compounds able to show different redox states that arevery appealing candidates to be used as wires and/or switches inmolecular electronics. In this regard, molecules having redoxcenters such as viologen [5,6], aniline [7,8], thiophene ,anthraquinone  and ferrocene  have been previouslystudied. However, a particularly suitable redox-active moleculefor molecular electronics is the well-known electron donortetrathiafulvalene (TTF) molecule. Pristine TTF, as well as thetetraselenafulvalene analogue (TSF), have been previouslyreported. In this study, the authors hypothesized that in theAuTTFAu junctions, the molecule is connected to the elec-trodes in a face-to-face overlapping configuration . Incontrast, since the first report on a suitably functionalized TTFas a molecular wire using two thioacetate anchoring groups, most of the TTF derivatives synthesized for this purposehave been functionalized with sulfur atoms as alligator clips.These belong either to a fused ring on the TTF , or to achain covalently connected to the TTF core bearing a thiolgroup at the end [15,16]. Furthermore, extended TTF cruciformmolecules, formed by two orthogonally placed, -conjugatedmoieties bearing the 1,3-dithiole rings at the ends, have alsobeen used for single-molecule measurements .
A singular TTF analogue is the so-called -extended TTF(exTTF, (9,10-bis(1,3-dithiol-2-ylidene)-9,10-dihydroanthra-cene) which, in contrast to pristine TTF that exhibits two oxi-
dation peaks to form the radical cation and dication species,shows only one oxidation peak involving a two electron processto form the dication state. Furthermore, the geometrical prop-erties of exTTF are quite different from pristine TTF. Thus,whereas TTF is mostly planar in the neutral form, exTTF is ahighly distorted, out-of-plane molecule with a butterfly shape inits neutral state. It undergoes a dramatic gain of planarity andaromaticity upon oxidation (Figure 1) [18,19]. This gain ofstability upon oxidation has been skillfully used in a variety ofDA systems, namely exTTF-bridgeC60 derivatives, fordetermining the attenuation factor of the molecular wire(oligomer) acting as the -bridge [20-22].
Figure 1: Depictions of 9,10-bis(1,3-dithiol-2-ylidene)-9,10-dihydro-anthracene (exTTF) in the (a) neutral form and (b) in the oxidized (2+)state. In the oxidized state the two positive charges reside on the two1,3-dithiole rings.
In this paper, we describe the synthesis of a new exTTF deriva-tive, suitably functionalized with two (p-acetylthio)phenyl-ethynyl substituents at positions 2 and 6 of the anthracenecentral core. We then describe single-molecule conductancemeasurements on this new derivative, along with measure-ments of the charge-transfer complex formed with F4TCNQ.Finally, we present theoretical calculations to understand itselectrical transport properties.
Results and DiscussionSynthesis and characterization of molecularwire 5The synthesis of the target molecule is shown in Scheme 1 andstarts from the previously reported 2,6-diiodo-exTTF 1 .Reaction of 1 under Sonogashira conditions (Pd(II), CuI,DIPEA) with trimethylsilylacetylene affords the symmetricallysubstituted exTTF 2 in good yield. Further removal of thetrimethylsilyl group is easily achieved by treatment with potas-sium carbonate, yielding the free terminal alkyne 3 in quantitat-ive yield. The introduction of the two anchor groups in 3 iscarried out through a second Sonogashira reaction. Thecoupling of 2,6-diethynyl-exTTF 3 with 1-acetylthio-4-iodoben-
Beilstein J. Org. Chem. 2015, 11, 10681078.
Scheme 1: Synthetic route to the target exTTF-based molecular wire 5.
zene (4), in the presence of Pd(II) and copper iodide and DIPEAin THF, led to the target molecule 5 in moderate yield (35%).Compound 4 was obtained in one step and with high yield from1,4-diiodobenzene by reaction with n-BuLi in ether, followedby reaction with S8, and eventually, acetyl chloride .
All new compounds were fully characterized by spectroscopicand electrochemical means. Interestingly, compounds 2, 3 and 5showed similar 1H NMR spectra due to their symmetry result-ing in relatively simple spectra, which confirms the proposedstructures. In particular, compound 5 exhibits the methyl groupsas a singlet at 2.45 ppm, and the protons corresponding to the1,3-dithiole rings appear as a singlet at 6.37 ppm. In the13C NMR of the target molecule 5, the carbonyl groups appearat 192.4 ppm and the carbons of the alkyne moieties at 88.0 and90.4 ppm, with the terminal methyl groups at 28.7 ppm.
The redox properties of compound 5 (0.2 mM) were deter-mined by cyclic voltammetry at room temperature in THF usingTBAPF6 (0.1 M) as a supporting electrolyte under argon atmos-phere and at a scan rate of 0.1 Vs1. The electrochemical cellconsisted of a glassy carbon working electrode, Ag/AgNO3reference electrode and a Pt wire counter electrode. It is worthmentioning that ferrocene was not employed as the inner refer-ence since its oxidation potential overlaps with that of theexTTF unit. Similar to pristine exTTF, the new exTTF deriva-tive 5 exhibited only one quasi-reversible oxidation peak,involving a two-electron process to form the dication state[25,26]. This oxidation peak appears at Epa = 217 mV(E = 285 mV, peak-to-peak separation), which is quite similar
to the oxidation peak found for pristine exTTF (Epa = 244 mV,E = 350 mV) (Figure 2).
Figure 2: Cyclic voltammograms of compound 5 and pristine exTTF(at concentrations of approximately 0.2 mM) using THF as a solventand TBAPF6 (0.1 M) as a supporting electrolyte. Scan rate: 0.1 Vs1.
Break junction measurementsNeutral moleculeWe first tried to form neutral-molecule molecular junctions.Simply, compound 5 can be seen as an analogue of anoligo(phenylene ethynylene), specifically an OPE3-dithiol com-pound (where 3 indicates the total number of phenyl rings), inwhich the central phenyl ring has been substituted by an exTTFunit. We could, therefore, expect compound 5 to form molec-ular junctions in a similar way to the OPE3-dithiol, which
Beilstein J. Org. Chem. 2015, 11, 10681078.
readily does so either in solution, or under solvent-free condi-tions as recently reported . Hence, as a starting point, wefollowed the same sample preparation conditions as previouslywith the OPE3-dithiol . We prepared 0.11 mM solutions ofcompound 5 in both 1,2,4-trichlorobenzene (TCB) or mesity-lene/tetrahydrofuran (Mes/THF 4:1), and exposed a clean goldsubstrate to the solution for a period of approximately 30 min.The sample was then dried under a flow of argon and mountedinside the scanning tunneling microscope (STM). All experi-ments were then performed under solvent-free, ambient condi-tions. In order to form molecular junctions of compound 5, wefollowed the break junction technique . During the experi-ment, the variation in conductance (G) is recorded while anSTM tip is moved vertically (z) in and out of contact with agold substrate, forming and breaking gold nanocontacts (G vs ztrace). When the two gold electrodes (the STM tip and the sub-strate) are in contact, or in close enough proximity, one or moremolecules of the compound adsorbed on the surface can bridgethe two electrodes. This binding occurs through one of theterminal groups (thiols in this case) to each of the electrodes,hence forming a molecular junction. In this configuration, whenseparating the electrodes (larger z values), we observe conduc-tance plateaus while the gold nanocontact or a molecular junc-tion remains intact during the pulling. The plateaus then endabruptly when the junction is broken.
Figure 3c and 3d show the 2D histograms consisting of severalthousand individual G vs z traces recorded in a break junctionexperiment in the presence of compound 5. These are comparedwith those recorded on an unmodified gold substrate and in thepresence of OPE3-dithiol. These histograms include all themeasured traces without filtering out the tunneling-only tracesfrom those with plateaus. One can see that the colored region ofthe 2D histogram of OPE3-dithiol extends significantly to largerinter-electrode distances than the unmodified gold substrate.Also, it does so within a narrow band of conductance values(roughly between log(G/G0) = 3 and 4.5). This 2D profileexemplifies the presence of plateaus occurring in a narrowregion of conductance. In the 2D histograms of compound 5, wecan also see that the colored region extends to higher electrodeinterdistance values (z) than for the unmodified gold substrate.However, as opposed to the case of OPE-dithiol, there is noclear protuberance in the histogram that would indicate theconcentration of plateaus at a given conductance value.
Therefore, in order to determine whether the signature of com-pound 5 is simply very weak, we performed a trace separationprocess to build histograms of only the traces displayingplateaus. Figure 4 shows the results of this separation for thetraces considered in Figure 3. In particular, for compound 5,two separation steps were carried out, resulting in three cate-
Figure 3: 2D histograms resulting from break junction experiments onan unmodified gold sample (a), OPE3-dithiol drop-cast from TCB (26%of traces displayed plateaus around 104 G0) (b), compound 5 drop-cast from TCB (c) and, compound 5 dip-cast from dichloromethane (d).All measurements were performed in dry ambient conditions.
gories of traces: (1) those with only a smooth exponential decay(Figure 4a and Figure 4d, labeled No Plat.), (2) those withpoorly-defined plateaus (Figure 4b and Figure 4e, labeled Plat.1), and (3) those with well-defined plateaus (Figure 4c andFigure 4f, labeled Plat. 2). We considered the conductancerange between log(G/G0) = 5.3 and 0.5 and established that atrace has a plateau whenever a z interval (z) longer than0.15 nm is needed to observe a change of conductancelog(G/G0) = 0.12 along the trace. Amongst these traces, weseparate the well-defined plateaus as those traces for which a zlarger than 0.2 nm is needed to observe a log(G/G0) = 0.1along the trace. These are empirical criteria which gave us thebest separation results. We see that the histograms built fromthe trace of the third group present protuberances, suggestingthat molecular junctions are successfully formed fromcompound 5.
From a close inspection of Figure 4c and Figure 4f, we see thatthe plateau conductance in these experiments varies by morethan 2 orders of magnitude (between log(G/G0) = 3 and 5),significantly greater than OPE3-dithiol, and also that theyextend to between 1 and 2 nm. However, it is important to notehere that the percentage of traces with well-defined plateaus(given in parentheses in Figure 4) is very low. Even with a totalnumber of 5000 measured traces, the final number of traces
Beilstein J. Org. Chem. 2015, 11, 10681078.
Figure 4: 2D histograms corresponding to compound 5 after exposing a gold substrate to the solution of the compound in TCB. For each measure-ment, the traces were separated into 3 groups: traces with no plateau (No Plat.), traces with poorly defined plateaus (Plat. 1), and traces with well-defined plateaus (Plat. 2). See text for details on the separation process. The percentage of traces included in each group is indicated in the brackets.
Figure 5: 2D histograms corresponding to compound 5 after exposing a gold substrate to a solution of the compound in DCM. The traces were sep-arated into three groups as described in Figure 4. The total number of traces recorded was 3830.
with well-defined plateaus is less than 50 traces. We also notehere that these results correspond to the most successfulmeasurement runs, and the percentage of traces with plateauswas even lower in other cases. We stress that under the sameexperimental conditions, we obtained percentages of around35% of well-defined plateaus for OPE3-dithiol.
We have recently measured the conductance of a series of mole-cules based on a similar OPE3 backbone, also terminated withthiols, but with differing numbers of dithiafulvalene (DTF)substituents placed at various positions along the OPE back-bone . One of the main structural differences with thesemolecules compared to compound 5 is that conjugation is main-
tained along the OPE3 backbone. For this series of compounds,we could observe a clear signature for each, which was similarto the unmodified OPE3. We showed that the presence of theDTF side groups does not influence the low-bias conductanceand secondly, and that their presence does not significantlyhinder molecular junction formation. Different to the measure-ments carried out thus far on compound 5, we carried out thesemeasurements using dichloromethane as the deposition solvent,and since the results were clear, we decided to applied this alsoto compound 5. The sample was prepared by exposing the goldto a solution of compound 5 in dichloromethane (DCM) for 1 h,followed by drying the sample with a flow of N2. The results ofthese measurements are shown in Figure 5.
Beilstein J. Org. Chem. 2015, 11, 10681078.
As with the measurements on compound 5 using the TCB drop-casting method, after dip-casting from DCM, we could observethe presence of G(z) plateaus, in this case down to just above107 G0 facilitated by the use of larger gains. The percentage oftraces displaying these plateaus was again low, however, andsimilar to that found before, with less than 2% fitting the well-defined criteria. From the 2D histograms in Figure 4, we seeagain that no favored region of conductance develops afterseparating the junctions displaying plateaus (labeled Plat. 1 andPlat. 2). This, we believe, indicates that whilst the formation ofmolecular junctions is possible, it is unclear exactly how themolecule binds in these junctions. The low percentage of mole-cular junction formation can be considered consistent with ourobservations on the OPE3 series with DTF side groups, in thatthe presence of sulfur atoms in the center of the moleculeslightly reduces the probability of forming junctions. This islikely because the mobility of the molecule over the surface isreduced, which in turn makes it difficult for molecules todiffuse into the freshly created nanogaps.
The lack of a clear molecular signature may ultimately be due toseveral reasons. Aside from reducing the probability of junc-tion formation, the sulfur atoms in the center of the moleculecan also bind to the electrodes during the evolution of the junc-tions, preventing the wire from becoming fully stretched. Thisis a distinct possibility for this molecule due to the well-knowninteraction of the parent extended-TTF and gold . An alter-native explanation for the lack of a clear signal for compound 5is that its end-to-end conductance is too low for it to beobserved in our setup. If this is the case, this would mean theconductance is lower than 107 G0. This is quite likely due tothe cross-conjugated nature of the exTTF unit, and the knowneffect this has on conductance.
Conductance measurements on the exTTF-F4TCNQ charge-transfer complexDespite the lack of a clear signal for the neutral molecule, wedecided to proceed by trying to form the charge-transfer (CT)complex of compound 5 with 7,7,8,8-tetracyanoquinodi-methane (TCNQ). When combining two equimolar solutions ofthe two compounds in DCM, we observed no color change,suggesting no complexation. The solvent was then changed toacetonitrile, a more polar solvent better able to stabilize com-plex formation, but this too did not give the anticipated strongcolor change. Only when the solution was heated at reflux for3 h under ambient conditions and a large excess of TCNQ wasadded (5 equiv), a dark green color developed. UVvis absorp-tion spectroscopy confirmed the formation of a CT complex(Supporting Information File 1, Figure S1). To ensure the quan-titative formation of the CT complex, a more straightforwardmethod compatible with the conductance measurements was
considered. Specifically, we switched from TCNQ to thestronger acceptor 2,3,5,6-tetrafluoro-7,7,8,8-tetracyanoquinodi-methane (F4TCNQ). This produced a clear change of color assoon as the first drops of the acceptor were added to the solu-tion of compound 5 in DCM, yielding a green solution. Wemonitored the formation of the CT complex by recording theUVvis spectrum of the solution. As successive amounts of theacceptor are added to the solution of the donor, the peak at448 nm of the neutral donor species decreases and new peaksappear between 600900 nm that grow with the addition ofmore acceptor and also methanol (see Supporting InformationFile 1, Figure S2). Specifically, we observe three peaks at689 nm, 764 nm and 867 nm, which can be assigned to theradical anion F4TCNQ species . For the break junctionmeasurements, it was necessary to avoid having an excess ofthe acceptor because F4TCNQ forms molecular junctions itselfdue to its four terminal cyano groups (see Supporting Informa-tion File 1, Figure S7). Hence, we formed the charge-transfer(CT) complex by adding approximately 0.5 mL of a 104 Msolution of F4TCNQ in DCM to a 1 mL 104 M solution ofcompound 5. In this way, we can avoid having significantamounts of free acceptor on the surface. This, however, meanswe do not exactly know the ratio of donor to acceptor in ourcase. It is known that the CT complex of the parent exTTF withTCNQ forms in a 1:4 ratio . However, as we have evidenceof the formation of a radical anion of F4TCNQ, we believe adonor to acceptor ratio of 1:2 is more likely, for which there is aprecedent in a substituted exTTF complex with TCNQ . Wethen allowed 24 h for the molecules to adsorb onto the gold inorder to obtain as high a density of molecules as possible. Thisincreases the possibility that a significant fraction of the solu-tion is still the free donor species. Although there will still besome of the neutral donor species present on the surface, as wehave shown that this molecule does not give a clear signal inbreak junction experiments, there will be no problem of signaloverlap with the CT complex.
In contrast to the neutral form of compound 5, a significantpercentage of conductance plateaus for the CT complex samplewere observed. They were found fall into two main groups,labeled as high and low conductance. Figure 6a shows exam-ples of individual G(z) traces displaying conductance plateaus.Firstly, we separate traces showing only tunneling (Figure 6b)from those containing plateaus (Figure 6c) using the followingcriteria: z interval (z) longer than 0.12 nm needed to observe achange of conductance log(G/G0) = 0.16. We then furtherdivided the traces into two more groups for those with plateausabove or below log(G/G0) = 3.8. Dividing the traces using avalue slightly above or below this does not change the sep-aration significantly as the difference between the two types ofplateaus is clear. By fitting a Gaussian function to the
Beilstein J. Org. Chem. 2015, 11, 10681078.
Figure 6: a) Examples of individual G(z) traces showing clear conductance plateaus. be) 2D histograms corresponding to the CT complex betweencompound 5 and F4TCNQ after exposing a gold substrate to the solution of the complex in DCM. The traces are separated into four groups: b) traceswithout plateaus; c) traces with plateaus between log(G/G0) = 0.5 and 6.0. From these traces the traces were divided into high and low plateaugroups: d) traces with plateaus above log(G/G0) = 3.8; e) traces with plateaus below log(G/G0) = 3.8. The total number of traces recorded was4868.
histograms we find peak positions of log(G/G0) = 3.0 forthe high group, and log(G/G0) = 4.7 for the low group (seeSupporting Information File 1, Figure S6 for the 1Dhistograms). We also measured the junction break-off distancefor the two groups (which we define as the separation requiredto move from log(G/G0) = 0.5 to either log(G/G0) = 4 for thehigh plateaus, or log(G/G0) = 6.1 for the low plateaus). Wefound mean values of 0.65 0.25 nm and 1.14 0.30 nm forthe high and low groups, respectively (see Supporting Informa-tion File 1, Figure S3 for break-off histograms). We repeatedthe measurements using a freshly prepared CT complex andgold electrodes, and obtained a very similar result for the lowconductance group (see Supporting Information File 1, FiguresS4 and S5). In the repeated measurement, however, we did notobserve a signal in the high conductance region, above 103 G0.
As can be seen from the separation of plateaus into high andlow groups, the two types generally occur independently. Theorigin of the high conductance state is difficult to be totally sureabout. The two groups may arise from independent chemicalspecies, in which case it would be natural to label the highgroup as junctions for which transport takes place through a
molecule of F4TCNQ. The length and conductance are similarto the control test we carried out on only this molecule (seeSupporting Information File 1, Figure S7). It may also bepossible that the high conductance state arises through contactto the central part of the CT complex and one of the terminalthiol groups. We observed a similar feature for the neutralmolecule (see Figure 4b and Figure 4c) although for the neutralmolecule, this signal was never very reproducible. The lowgroup, on the other hand, fits well with conductance takingplace across the whole molecule (i.e., thiol to thiol). We calcu-late an SS distance of 2.4 nm for the CT complex (substitutingthe dihydroanthracene core of compound 5 for anthracene). Weestimate the amount of gold retraction to be 0.5 nm, which thengives a real AuAu separation of 1.64 0.30 nm for the meanbreaking distance of the low group, corresponding well with thelength of the molecule. The fact that the molecule does notseem to fully stretch inside the junctions (unlike the OPE3-dithiol) may be due to the bulky nature of the complex, whichcontains many groups with the potential to interact with gold.
We cannot be totally sure of the species which gives rise to thelow conductance state in so much as we do not know its exact
Beilstein J. Org. Chem. 2015, 11, 10681078.
charge and ratio of donor to acceptor molecules. It is conceiv-able that some charge is transferred to the electrodes uponmolecular junction formation, as is common for molecular junc-tions . However, it is well known that the cationic (1+) stateof exTTF is less thermodynamically stable than the dication(2+) , resulting in inverted oxidation potentials of the cationand dication. Additionally, it is known that the resonancebetween the neutral and dication is impossible due to the strongdifference in geometries. Thus, it is more than plausible that themolecule retains its cationic state in the junction. We furtherpoint out that in several recent studies, a very similar conduc-tance was found for a molecule that is structurally similar andcontains only the anthracene central group. In a study by Honget al., a conductance peak was found at log(G/G0) = 4.5, whichis close to the low conductance group we observe . As it isknown that the oxidation of exTTF compounds results in theplanarization and aromatization of the central three rings to theanthracene unit, the similarity in conductance is perhaps indica-tive of these changes. We have also recently shown that addingsubstituents to the central phenyl rings of OPE wires has nonoticeable influence on the molecular conductance (groupswere tested ranging from electron-withdrawing fluorine to elec-tron-donating methoxy groups) . It is also rational tosuppose that the, albeit charged, dithiole side groups of our CTcomplex would not strongly modify the conductance of theotherwise neutral anthracene-containing wire. Finally, we pointout that recent conductive AFM measurements carried out onself-assembled monolayers of anthracene and anthraquinoneOPE derivatives showed a difference of approximately twoorders of magnitude between their respective conductancevalues . This would fit with our hypothesis that the conduc-tance of the neutral exTTF molecule, which has a similarbonding pattern to anthraquinone, is below our experimentalresolution, based on the value we measure for the CT complex.
Ab initio calculationsTo gain insight into the conduction mechanism of compound 5,we performed theoretical calculations based on a combinationof density functional theory (DFT) and Greens functions tech-niques within the framework of the Landauer theory forcoherent transport. The complete technical details are reportedin Supporting Information File 1.
We first optimized the geometry of the molecule in the gasphase. The HOMO was found to be localized on the exTTFunit, which presented the expected butterfly shape, whilethe LUMO appeared delocalized over the whole molecule(Figure 7).
Subsequently, we constructed two kinds of metalmole-culemetal junctions, where the molecule is bound to a gold
Figure 7: Frontier orbitals of compound 5 in the gas phase.
cluster in a top and hollow position, respectively (Figure 8). Wethen computed the zero-bias electron transmission following theprocedure explained in Supporting Information File 1. Thecorresponding transmission curves are shown in Figure 9.Notice that the molecular HOMOLUMO gap was corrected,following the procedure previously reported . TheHOMO and all other occupied orbital energies were shifted byocc=IP H +occ, while the LUMO and all other unoccu-pied orbital levels were shifted by virt=EA L +virt. Here,occ (virt) is the image charge correction for the occupied(unoccupied) states, H (L) is the KohnSham energy of thegas phase HOMO (LUMO), and IP(EA) is the gas phase ioniza-tion potential (electron affinity). All quantities are reported inTable 1 for both binding geometries.
The alignment of the BreitWigner resonances related to boththe HOMO and LUMO (at approximately 1 and 2.7 eV fromthe Fermi level, respectively) do not show a strong dependenceon the binding geometry (Figure 9). The electron transport isdominated by the HOMO, although interference features (reso-nanceantiresonance pairs) appear in the energy region close tothe Fermi level. This is not surprising, given the spatial exten-sion of the frontier orbitals, in particular of the HOMO, whichis localized on the ex-TTF unit only. In fact, Fano resonancesare known to arise when a pendant orbital, which is weaklycoupled to the electrodes, is coupled to an orbital delocalizedover the main axis of the molecular wire [38,39].
Beilstein J. Org. Chem. 2015, 11, 10681078.
Figure 8: Top a) and hollow b) binding geometries of 5 to a gold cluster in metalmoleculemetal junctions.
Figure 9: Transmission as a function of energy for the top and hollowbinding geometries.
Table 1: KohnSham HOMO and LUMO, ionization potential (IP),electron affinity (EA) and image charge correction for occupied occand virt unoccupied orbitals. All quantities are in eV.
HOMO IP occ LUMO EA virt
top 4.27 5.68 0.35 2.54 1.16 0.38hollow 4.27 5.68 0.32 2.54 1.16 0.33
The computed conductance values, evaluated as the transmis-sion at the Fermi level, are in the range 106 to 107 G0. Theselow conductance values are at the limit of what we can observeexperimentally. This, therefore, would be consistent with the
idea that the real conductance of the molecule is too low to berecorded in the experiments. Nevertheless, we cannot absolutelyrule out the possibility that the molecule does not form molec-ular junctions in the experiments.
ConclusionWe have synthesized a molecular wire containing a -extendedtetrathiafulvalene (exTTF) group and studied its single-mole-cule electrical transport properties along with those of itscharge-transfer complex with F4TCNQ. Within the accessibleconductance range (10 to 107 G0) we did not observe a clearconductance signature of the neutral parent molecule. Thisalone could suggest either that its conductance is too low or thatit does not form stable junctions. We did, however, find a clearconductance signature in the experiments carried out on thecharge-transfer complex. As complexation with the acceptoroxidizes the molecule by removing two electrons from theexTTF group, thus converting it from a buckled and cross-conjugated group into a planar aromatic group, we predict theCT species to have a higher conductance than the neutral mole-cule. This, we believe, supports the idea that the conductance ofthe neutral molecule is very low, below our measurement sensi-tivity. This would make the conductance difference between theneutral and CT species at least two orders of magnitude. Thiscan be considered as favorable for the use of single moleculesas chemical sensors, in which analyte molecules may bind to abackbone to alter its conductance. Further combinations ofdonors and acceptors should be explored in order to evaluatethis potential.
Beilstein J. Org. Chem. 2015, 11, 10681078.
Supporting InformationSupporting Information File 1Detailed experimental procedures for the synthesis andcharacterization of 5, break junction experiments andtheoretical methods.[http://www.beilstein-journals.org/bjoc/content/supplementary/1860-5397-11-120-S1.pdf]
AcknowledgementsWe thank Dr. Jose Manuel Santos Barahona for help with pre-paring the CT complex with TCNQ, and recording and inter-preting the UVvis spectra. Financial support by the EuropeanCommission (EC) FP7 ITN MOLESCO Project No. 606728,the European Resea rch Counc i l (ERC-436 2012ADG_20120216-Chirallcarbon), the CAM (PHOTOCARBONproject S2013/MIT-2841, NANOFRONTMAG-CM projectS2013/MIT-2850 and MAD2D project S2013/MIT-3007), FP7-ENERGY-2012-1-2STAGE-number 309223 (PHOCS) and theSpanish MICINN/MINECO through the programs MAT2011-25046, MAT2014-57915-R and PRI-PIBUS-2011-1067 isacknowledged. MB was partly supported by a FY2012(P12501) Postdoctoral Fellowship for Foreign Researchers fromthe Japan Society for Promotion of Science (JSPS) and by aJSPS KAKENHI, Grant-in-Aid for JSPS Fellows, grant no.2402501. YA is also thankful to another KAKENHI, Grant-in-Aid for Scientific Research on Innovation Areas, MolecularArchitectonics: Orchestration of Single Molecules for NovelFunctions (#25110009). LAZ was supported by the SpanishMICINN under Grant MAT2011-23627. FP acknowledgessupport by the Carl-Zeiss foundation and the CollaborativeResearch Center 767 Controlled Nanosystems: Interaction andInterfacing to the Macroscale.
References1. Leary, E.; La Rosa, A.; Gonzlez, M. T.; Rubio-Bollinger, G.; Agrat, N.;
Martn, N. Chem. Soc. Rev. 2015, 44, 920942.doi:10.1039/C4CS00264D
2. Guldi, D. M.; Nishihara, H.; Venkataraman, L., Eds. Molecular wires.Chem. Soc. Rev. 2015, 4, 8351030. doi:10.1039/C5CS90010G
3. Forrest, S. R.; Thompson, M. E., Eds. Organic Electronics andOptoelectronics. Chem. Rev. 2007, 107, 9231386.doi:10.1021/cr0501590
4. Guldi, D. M.; Illescas, B. M.; Atienza, C. M.; Wielopolski, M.; Martn, N.Chem. Soc. Rev. 2009, 38, 15871597. doi:10.1039/b900402p
5. Haiss, W.; van Zalinge, H.; Higgins, S. J.; Bethell, D.; Hbenreich, D.;Schiffrin, D. J.; Nichols, R. J. J. Am. Chem. Soc. 2003, 125,1529415295. doi:10.1021/ja038214e
6. Gittins, D. I.; Bethell, D.; Schiffrin, D. J.; Nichols, R. J. Nature 2000,408, 6769. doi:10.1038/35040518
7. Chen, F.; He, J.; Nuckolls, C.; Roberts, T.; Klare, J. E.; Lindsay, S.Nano Lett. 2005, 5, 503506. doi:10.1021/nl0478474
8. Chen, F.; Nuckolls, C.; Lindsay, S. Chem. Phys. 2006, 324, 236243.doi:10.1016/j.chemphys.2005.08.052
9. Xu, B. Q.; Li, X. L.; Xiao, X. Y.; Sakaguchi, H.; Tao, N. J. Nano Lett.2005, 5, 14911495. doi:10.1021/nl050860j
10. Hong, W.; Valkenier, H.; Mszros, G.; Manrique, D. Z.;Mishchenko, A.; Putz, A.; Moreno Garca, P.; Lambert, C.;Hummelen, J. C.; Wandlowski, T. Beilstein J. Nanotechnol. 2011, 2,699713. doi:10.3762/bjnano.2.76
11. Xiao, X.; Brune, D.; He, J.; Lindsay, S.; Gorman, C. B.; Tao, N.Chem. Phys. 2006, 326, 138143.doi:10.1016/j.chemphys.2006.02.022
12. Taniguchi, M.; Tsutsui, M.; Shoji, K.; Fijiwara, H.; Kawai, T.J. Am. Chem. Soc. 2009, 131, 1414614147. doi:10.1021/ja905248e
13. Giacalone, F.; ngeles Herranz, M.; Grter, L.; Gonzlez, M. T.;Calame, M.; Schnenberger, C.; Arroyo, C.; Rubio-Bollinger, G.;Vlez, M.; Agrat, N.; Martn, N. Chem. Commun. 2007, 48544856.doi:10.1039/b710739k
14. Li, M.-J.; Long, M.-Q.; Chen, K.-Q.; Xu, H. Solid State Commun. 2013,157, 6267. doi:10.1016/j.ssc.2012.12.001
15. Leary, E.; Higgins, S. J.; van Zalinge, H.; Haiss, W.; Nichols, R. J.;Nygaard, S.; Jeppesen, J. O.; Ulstrup, J. J. Am. Chem. Soc. 2008, 130,1220412205. doi:10.1021/ja8014605
16. Liao, J.; Agustsson, J. S.; Wu, S.; Schnenberger, C.; Calame, M.;Leroux, Y.; Mayor, M.; Jeannin, O.; Ran, Y.-F.; Liu, S.-X.; Decurtins, S.Nano Lett. 2010, 10, 759764. doi:10.1021/nl902000e
17. Parker, C. R.; Leary, E.; Frisenda, R.; Wei, Z.; Jennum, K. S.;Glibstrup, E.; Abrahamsen, P. B.; Santella, M.; Christensen, M. A.;Della Pia, E. A.; Li, T.; Gonzlez, M. T.; Jiang, X.; Morsing, T. J.;Rubio-Bollinger, G.; Laursen, B. W.; Nrgaard, K.; van der Zant, H.;Agrat, N.; Nielsen, M. B. J. Am. Chem. Soc. 2014, 136, 1649716507.doi:10.1021/ja509937k
18. Martn, N.; Snchez, L.; Herranz, M. A.; Illescas, B.; Guldi, D. M.Acc. Chem. Res. 2007, 40, 10151024. doi:10.1021/ar700026t
19. Brunetti, F. G.; Lpez, J. L.; Atienza, C.; Martn, N. J. Mater. Chem.2012, 22, 41884205. doi:10.1039/c2jm15710a
20. Giacalone, F.; Segura, J. L.; Martn, N.; Guldi, D. M. J. Am. Chem. Soc.2004, 126, 53405341. doi:10.1021/ja0318333
21. Molina-Ontoria, A.; Wielopolski, M.; Gebhardt, J.; Gouloumis, A.;Clark, T.; Guldi, D. M.; Martn, N. J. Am. Chem. Soc. 2011, 133,23702373. doi:10.1021/ja109745a
22. Wielopolski, M.; Molina-Ontoria, A.; Schubert, C.; Margraf, J. T.;Krokos, E.; Kirschner, J.; Gouloumis, A.; Clark, T.; Guldi, D. M.;Martn, N. J. Am. Chem. Soc. 2013, 135, 1037210381.doi:10.1021/ja401239r
23. Illescas, B. M.; Santos, J.; Martn, N.; Atienza, C. M.; Guldi, D. M.Eur. J. Org. Chem. 2007, 50275037. doi:10.1002/ejoc.200700226
24. Pearson, D. L.; Tour, J. M. J. Org. Chem. 1997, 62, 13761387.doi:10.1021/jo962335y
25. Liu, S.-G.; Prez, I.; Martn, N.; Echegoyen, L. J. Org. Chem. 2000, 65,90929102. doi:10.1021/jo001149w
26. Herranz, M. A.; Yu, L.; Martn, N.; Echegoyen, L. J. Org. Chem. 2003,68, 83798385. doi:10.1021/jo034894s
27. Gonzlez, M. T.; Leary, E.; Garca, R.; Verma, P.; Herranz, M. A.;Rubio-Bollinger, G.; Martn, N.; Agrat, N. J. Phys. Chem. C 2011, 115,1797317978. doi:10.1021/jp204005v
28. Chen, F.; Tao, N. J. Acc. Chem. Res. 2009, 42, 429438.doi:10.1021/ar800199a
Beilstein J. Org. Chem. 2015, 11, 10681078.
29. Urban, C.; cija, D.; Wang, Y.; Trelka, M.; Preda, I.; Vollmer, A.;Lorente, N.; Arnau, A.; Alcam, M.; Soriano, L.; Martn, N.; Martn, F.;Otero, R.; Gallego, J. M.; Miranda, R. J. Phys. Chem. C 2010, 114,65036510. doi:10.1021/jp911839b
30. Jain, A.; Rao, K. V.; Mogera, U.; Sagade, A. A.; George, S. J.Chem. Eur. J. 2011, 17, 1235512361. doi:10.1002/chem.201101813
31. Bryce, M. R.; Moore, A. J.; Hasan, M.; Ashwell, G. J.; Fraser, A. T.;Clegg, W.; Hursthouse, M. B.; Karaulov, A. I.Angew. Chem., Int. Ed. Engl. 1990, 29, 14501452.doi:10.1002/anie.199014501
32. Bryce, M. R.; Finn, T.; Batsanov, A. S.; Kataky, R.; Howard, J. A. K.;Lyubchik, S. B. Eur. J. Org. Chem. 2000, 11991205.doi:10.1002/1099-0690(200004)2000:73.0.CO;2-F
33. Peng, G.; Strange, M.; Thygesen, K. S.; Mavrikakis, M.J. Phys. Chem. C 2009, 113, 2096720973. doi:10.1021/jp9084603
34. Bendikov, M.; Wudl, F.; Perepichka, D. F. Chem. Rev. 2004, 104,48914946. doi:10.1021/cr030666m
35. Gonzlez, M. T.; Zhao, X.; Manrique, D. Z.; Miguel, D.; Leary, E.;Gulcur, M.; Batsanov, A. S.; Rubio-Bollinger, G.; Lambert, C. J.;Bryce, M. R.; Agrat, N. J. Phys. Chem. 2014, 118, 2165521662.doi:10.1021/jp506078a
36. Gudon, C. M.; Valkenier, H.; Markussen, T.; Thygesen, K. S.;Hummelen, J. C.; van der Molen, S. J. Nat. Nanotechnol. 2012, 7,305309. doi:10.1038/nnano.2012.37
37. Zotti, L. A.; Brkle, M.; Pauly, F.; Lee, W.; Kim, K.; Jeong, W.; Asai, Y.;Reddy, P.; Cuevas, J. C. New J. Phys. 2014, 16, 015004.doi:10.1088/1367-2630/16/1/015004
38. Cuevas, J. C.; Scheer, E. Molecular electronics: An Introduction toTheory and Experiment; World Scientific Publishing Co Pte Ltd:Singapore, 2010; Vol. 1. doi:10.1142/7434
39. Lambert, C. J. Chem. Soc. Rev. 2015, 44, 875888.doi:10.1039/C4CS00203B
License and TermsThis is an Open Access article under the terms of theCreative Commons Attribution License(http://creativecommons.org/licenses/by/2.0), whichpermits unrestricted use, distribution, and reproduction inany medium, provided the original work is properly cited.
The license is subject to the Beilstein Journal of OrganicChemistry terms and conditions:(http://www.beilstein-journals.org/bjoc)
The definitive version of this article is the electronic onewhich can be found at:doi:10.3762/bjoc.11.120
AbstractIntroductionResults and DiscussionSynthesis and characterization of molecular wire 5Break junction measurementsNeutral moleculeConductance measurements on the exTTF-F4TCNQ charge-transfer complex
Ab initio calculations